1560

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 8, AUGUST 2000

Physical Mechanisms Limiting the Manufacturing Uniformity of Millimeter-Wave Power InP HEMT’s S. Krupenin, Roxann R. Blanchard, Member, IEEE, M. H. Somerville, Jesus A. del Alamo, Senior Member, IEEE, K. G. Duh, and P. C. Chao, Senior Member, IEEE

Abstract—We have developed a methodology to diagnose the physical mechanisms limiting the manufacturing uniformity of millimeter-wave power InAlAs/InGaAs HEMT’s on InP. A statistical analysis was carried out on dc figures of merit obtained from a large number of actual devices on an experimental wafer. correlation studies and principal component analysis of the results indicated that variations in Si delta-doping concentration introduced during molecular-beam epitaxy accounted for more than half of the manufacturing variance. Variations in the gate-source distance that is determined by the electron-beam alignment in the gate formation process were found to be the second leading source of manufacturing variance. The statistical methodology used in this work is suitable for continuous process yield diagnostics and improvement in a manufacturing environment.

I. INTRODUCTION

T

HE InP high electron mobility transistor (HEMT) is the leading contender for high-power high-efficiency millimeter-wave power amplifiers [1], [2]. As the InP HEMT technology matures, manufacturing issues come to the foreground. To date there has been little work on understanding the key factors affecting the manufacturing uniformity of these devices. Such a study has been hampered by the considerable amount of work that it takes to measure millimeter-wave power figures of merit. Manufacturing uniformity control and improvement is critical because high cost represents a significant road block in the development of millimeter-wave systems. In this work we have carried out a statistical study of dc figures of merit of InP power HEMT’s that strongly impact the millimeter-wave performance of these devices. All of the selected figures of merit were measured in actual devices. A statistical analysis of the results using a principal components analysis (PCA) was carried out. This analysis was instrumental in revealing the two dominant physical sources of variability in these figures of merit. The methodology used in this work can be easily implemented in a manufacturing environment for continuous process diagnostics and improvement.

Manuscript received August 6, 1999; revised February 2, 2000. This work was supported by the MAFET program, through Sanders Lockheed Martin. The review of this paper was arranged by Editor A. S. Brown. S. Krupenin is with Stanford University, Stanford, CA 94305 USA. R. R. Blanchard is with Analog Devices Inc., Wilmington, MA 01887 USA. M. H. Somerville is with Vassar College, Poughkeepsie, NY 12604 USA. J. A. del Alamo is with the Massachusetts Institute of Technology, Cambridge, MA 02139 USA (e-mail: [email protected]). K. G. Duh and P. C. Chao are with Sanders Lockheed Martin, Nashua, NH 03061 USA. Publisher Item Identifier S 0018-9383(00)06032-9.

II. EXPERIMENTAL The devices studied in this work are 0.1 m gate length and 25 m gate width double-heterostructure InP power HEMT’s on one experimental 3-in wafer from Lockheed Martin Sanders [3], [4]. The heterostructure was grown by molecular-beam epitaxy (MBE) and includes two Si delta-doped layers above and below the channel. The devices feature an electron-beam written T-gate and a selectively recessed depleted cap. A total of 50 devices located on every other die of the wafer were studied. All figures of merit were measured with an identical probe configuration, allowing fast and completely automated measurements. We selected ten dc figures of merit that map to key millimeter-wave power figures of merit. They are listed in Table I. They include the threshold voltage, , the maximum transcon, the gate-source voltage at which ductance, occurs, , the maximum drain current, , the output conductance, , the off- and on-state breakdown and , and the source and voltages, and . The measurement conditions for drain resistances, these figures of merit are also summarized in Table I. Basically, and were obtained from the transfer characteristics. was obtained from two transfer char. and acteristics at two close values of were extracted using the drain-current injection technique [5]. was measured using the gate-current extraction techand were obtained using the end-resistance nique [6]. technique [7]. Of the 50 devices that were measured two were found to be anomalous and their corresponding data were discarded. Table I lists the mean and standard deviation of each figure of merit. The standard deviation as percentage of the mean is additionally given. Variations of the figures of merit never exceed 16% across the entire wafer. The correlation matrix of the measurements of the figures of merit is shown on Fig. 1. Each vignette lists the correlation coefficient between two figures of merit. A correlation coefficient close to one indicates a strong positive correlation between the two selected figures of merit; if close to 1, the correlation is strong but negative; if close to zero, the correlation is weak. Some of the correlation coefficients on Fig. 1 can be interpreted and exhibit a strong positive cordirectly. For example, relation coefficient of 0.68. This suggests a contact resistance or doping level control problem and excludes misalignment of the gate process from being a dominant source of variation in these figures of merit (it would result in a negative correlation coefficient). Spatial information is often useful in identifying sources of variability. Fig. 2 shows the spatial distribution across the wafer

0018–9383/00$10.00 © 2000 IEEE

KRUPENIN et al.: MANUFACTURING UNIFORMITY OF MILLIMETER-WAVE POWER InP HEMT’s

DEFINITIONS

Fig. 1.

AND THE

1561

TABLE I MEASURED VALUES OF THE DC FIGURES OF MERIT USED IN THIS WORK (L = 0:1 m, “STDV” REFERS TO THE STANDARD DEVIATION OF THE FIGURES OF MERIT

W = 25 m).

Correlations among dc figures of merit. The number in each vignette indicates the correlation coefficient.

of two figures of merit: and . While exhibits a circular symmetry, appears to show a linear gradient from left to right in the figure. This suggests that there are at least two different and independent mechanisms at play that result in variations in the figures of merit. From examination of the data in Figs. 1 and 2 alone, it is not possible to uncover the physical sources of variability. In order

to further our insight into the physics underlying variations in the figures of merit we have performed PCA of the data. III. PRINCIPAL COMPONENT ANALYSIS PCA is a statistical technique that performs a coordinate transformation from the original space of electrical measure-

1562

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 8, AUGUST 2000

Fig. 2. Spatial distribution on the wafer of BV and g . The fact that these two distributions are very different suggests that there are at least two major mechanisms that result in manufacturing variations. Fig. 4. Contributions of each of the principal components to the variance of each dc figure of merit. The signs indicate whether a component has a positive or negative correlation with a given figure of merit (see text).

Fig. 3. Relative importance of the principal components in the manufacturing variance. P1 explains 51% of the variance of the manufacturing process.

ments to a new space of uncorrelated “principal components.” These principal components are ordered according to the total variance that they account for in the original data: first P1 is selected to account for the maximum possible variance in the data set, then the second component, P2, is selected to maximize the variance of the residual after P1 is removed, and so on. A comprehensive treatment of PCA can be found in [8]. More details about the use of PCA in our work can be found in [9]. In the first pass, all figures of merit were weighted equally. Emphasis on selected figures of merit can be made by introducing appropriate weights. The relative contribution of each principal component to the total variance of the data set is shown in Fig. 3. This figure shows that the most significant component, P1, accounts for 51% of the total variance of the process. Correct identification of this component followed by appropriate corrective action can significantly improve the manufacturing uniformity of this process. The second and the third components account for 21% and 13% of the total variance respectively. The rest of the components add up to a total of 15%. 80% confidence intervals for the contributions of each principal component can be found as in [8]. They are listed in brackets in Fig. 3. P1, for example, accounts with 80% confidence for 41% to 69% of the variance of the entire data set. The confidence intervals of components P5 through P10 overlap badly. This indicates that the experimental data is

insufficient for computing their values and identifying them. Identification and correction of the first three components, however, is sufficient for dramatic uniformity improvement. In order to carry out the identification of the leading principal components, their relative impact on each dc figure of merit should be examined. Fig. 4 shows a percentage of the variance of each figure of merit that is attributed to each principal component. For example, P1 accounts for nearly 80% of the variance of . In contrast, P1 accounts for less than 25% of the variance , while P2 accounts for nearly 70% of it. P3 is seen of to enter strongly in the variance of . The percentages shown in Fig. 4 are statistically significant for each of the three most important components. The standard deviations of the contributions of the first three principal components toward any figure of merit did not exceed 9% under the assumption of a multivariate normal distribution [8]. Hence Fig. 4 is a reliable vehicle for physical identification of the three leading principal components. Fig. 4 also indicates the sign of the correlation between the principal components and the figures of merit. PCA does not yield the absolute signs of the correlations, just the relative sign among all correlations of a given principal component. For exhas a contrary sign to ample, the correlation between P1 and . In Fig. 4, a choice of signs has the correlation of P1 and been made that makes physical sense and that aids the identification of the physical origin of the principal components. This is discussed in detail below. Spatial distributions of the principal components can also be constructed. They are exhibited on Fig. 5 for P1, P2 and P3. The circular symmetry of P1 and the linear gradient distributions of P2 and P3 offer further clues for their identification. This figure also shows how these three principal components are uncorrelated: their spatial distributions are very different. We now proceed to give a physical interpretation to P1, P2 and P3. The previous section suggests that these principal components are closely related to various steps of the manufacturing process. The identification is facilitated by Fig. 4, which indicates the nature of relationships between the principal components and the figures of merit.

KRUPENIN et al.: MANUFACTURING UNIFORMITY OF MILLIMETER-WAVE POWER InP HEMT’s

Fig. 5. Spatial distributions on the wafer of the first three principal components. Notice that the first component, P1, has a radial distribution, while P2 and P3 exhibit linear gradients along orthogonal directions.

A. Interpretation of P1 Fig. 4 shows that P1 has a strong positive correlation with and strong negative correlations with , the breakdown voltages, and the parasitic resistances. This behavior can only be explained by associating P1 with the sheet carrier concentration in the channel of the device, . Let us examine this hypothesis in detail. • P1 accounts for 78% of the variance in , and the correlaincreases the inversion charge tion is negative. Higher more negin the channel in equilibrium which makes ative. is large (77%) and positive. • The impact of P1 on in InP power This is consistent with the fact that [11]. HEMT’s is limited by • P1 has a relatively large impact on the variances of all three breakdown voltages, and the correlation between P1 and these quantities is negative. It is well known that all is increased these breakdown voltages decrease when [4], [10]. P1 accounts for a substantial fraction of the variance of and and exhibits a negative correlation. This is also consistent with P1 being related to in the channel since and is the access resistance from the a portion of edge of the ohmic contact to the edge of the gate. Additionally, this is a power device design with a surface depleted cap in which the access resistance is dominated by . • P1 has a small but positive correlation with the variance of . This is also consistent with the identification of P1 is the extrinsic transconductance as related to . increases through and it should increase slightly when on . the negative impact of The negative correlation between P1 and can be explained through the impact of on . As increases, shifts down and with it the whole vs. curve shifts to lower voltages, thus decreasing . and P1 stems from • The positive correlation between the fact that increases with the bias current at which it as discussed is measured which in turn increases with above. The preceeding discussion makes it quite convincing that P1 is directly associated with the sheet carrier concentration of change? There electrons in the channel, . But what makes

1563

are two possibilities for it, one is the InAlAs insulator thickness, the second one is the Si doping level in the delta-doped supply layers. The weak correlation between P1 and allows us to rule out the first option since a change in insulator thickness should strongly affect the transconductance of the device through the insulator capacitance. Hence, P1 represents the Si doping level in the supply layers. The Si dopants are introduced during the MBE growth of the structure in the form of two delta-doped layers above and below the channel. The sample is rotated during MBE growth in order to compensate for spatial nonuniformity of the Si flux emanating from the effusion cell. This compensation is not perfect and a variation of Si concentration with a circular symmetry results on the wafer. This is precisely what is observed for the spatial distribution of P1 over the wafer shown in Fig. 5. B. Interpretation of P2 P2 has a positive correlation with , but only a weak influ(Fig. 4). Its impact on is very large (63%), ence on but there is none on . There is also negligible influence of P2 on . This strongly suggests that P2 is related to the gatesource extrinsic region of the device. A likely explanation for the correlation of P2 with the figures of merit is the identifica. tion of P2 with the variations in the gate-source distance Let us examine this hypothesis in detail. , because does not • P2 has a negligible impact on depend on the position of the source contact relative to the gate. arises through • The negative correlation of P2 and , which is directly affected by . and • The negative correlations between P2, are related. The peak and subsequent drop in transconductance in the devices under test results from the blow up of source resistance at high current values due to velocity saturation [12]. A higher value of makes this condition occur at smaller values of current, and . thus leading to a smaller • As an extrinsic source related parameter, P2 should have no impact on and the breakdown voltages. makes sense • The positive correlation between P2 and is linearly proportional to . since is related to and that in turn is • In principle, since , one would expect a negative correlation affected by and P2: the higher , the smaller and between ought to be. This is not observed in our results. There and is no statistically significant correlation between P2. A possible explanation for this is that these are asymmetric devices with the gate placed closer to the source. Thus, the relative impact of misplacing the gate is significantly higher on the source side than on the drain side. Additionally, asymmetric gate placement makes the imthan , as observed in pact of variations higher in Fig. 4. This makes it harder to identify any other sources . of variance in Gate-source distance variations are determined by the reproducibility of the positioning of the electron beam process used to write the gate. P2 has a roughly linear distribution on the wafer

1564

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 8, AUGUST 2000

Fig. 6. Identity of the first two principal components in the structure of an InP power HEMT.

(Fig. 5). This is consistent with the identification of P2 as an electron-beam process related variable, since the electron beam draws the gate on the wafer scanning the die in a linear manner. Fig. 6 shows a schematic diagram of the device indicating the physical origin of P1 and P2. C. Interpretation of P3 , The results of Fig. 4 indicate that P3 affects only . This suggests a strong association of P3 with the exand trinsic drain portion of the device. Upon detailed examination of all correlations and their signs, no single structural parameter of the device could be found that is consistent with all results. The detailed origin of P3 remains unknown. IV. DISCUSSION Measurements on transmission line model (TLM) test structures were carried out in an effort to confirm the identity of P1. The saturation current that is obtained in a TLM structure when a relatively high voltage is applied is directly proportional to and the electron saturation velocity . Since is set by the nature of the material, it should not be affected by small manufacturing variations. Hence, the maximum current in a TLM constitutes a direct probe of the sheet carrier concentration in the channel of a HEMT with a depleted cap. The TLM’s used in this work were 100 m wide and 50 m long. The saturation current was measured at 10 V in every die in which transistor measurements had been performed. Fig. 7 , as a shows the obtained maximum current in each TLM, function of the value of P1 for every die. There is a very close correlation across the entire wafer in these two parameters: the correlation coefficient is 0.84. In consequence, this measurement constitutes an independent confirmation of the identification of P1 as the Si delta-doping concentration with a direct immade earlier. pact on the sheet carrier concentration Our findings are in substantial agreement with those of Elliott et al. [13] on TRW’s 3-in fabrication line for InP-based HEMT and HBT MMIC’s. These authors single out MBE growth as the most critical node in InP HEMT MMIC production. This is in agreement with the MBE origin of P1 in our work. Additionally, they identified gate formation as the second most critical node for HEMT’s. They found that gate length and gate-source spacing are critical parameters. While we have not been able to isolate the impact of the gate length variations, we relate P2 to

Fig. 7. Maximum current through a TLM test structure versus the P1 value for the HEMT device on the same die. The correlation coefficient is 0.84.

the distance between the gate and the source, in agreement with the findings in [13]. V. CONCLUSION In summary, we used PCA to identify the two most important sources of manufacturing variability in InP power HEMT’s: the concentration of Si dopants in the delta-doping layers of the device and the distance between the gate and the source. Jointly these two components account for 72% of manufacturing variations in this process. Our findings are in agreement with those reported by Elliott et al. [13] on TRW’s InP based MMIC fabrication line. Necessary statistical data were obtained from simple dc measurements on actual transistors—no specialized test structures were required. Our methodology can be easily implemented in a manufacturing environment for continuous process uniformity diagnostics and improvement. REFERENCES [1] P. M. Smith, “InP-HEMT’s for microwave and millimeter-wave applications,” in Int. Conf. InP and Related Materials, 1995, pp. 68–72. [2] J. A. del Alamo and M. H. Somerville, “Breakdown in millimeter-wave power InP HEMTs: A comparison with GaAs PHEMTs,” IEEE J. SolidState Circuits, vol. 34, pp. 1204–1211, Sept. 1999. [3] C. S. Putnam et al., “Temperature dependence of breakdown voltage in InAlAs/InGaAs HEMTs: Theory and experiments,” in Int. Conf. InP and Related Materials, 1997, pp. 197–200. [4] M. H. Somerville et al., “On-state breakdown in power HEMTs: Measurements and modeling,” in IEDM Tech. Dig., 1997, pp. 553–556. [5] S. R. Bahl and J. A. del Alamo, “A new drain-current injection technique for the measurement of breakdown voltage in FETs,” IEEE Trans. Electron Devices, vol. 40, pp. 1558–1560, Aug. 1993. [6] M. H. Somerville et al., “A new gate current extraction technique for measurement of on-state breakdown voltage in HEMTs,” IEEE Electron Device Lett., vol. 19, pp. 405–407, Nov. 1998. [7] K. Lee et al., “A new interpretation of “end” resistance measurements,” IEEE Electron Dev. Lett., vol. EDL-5, pp. 5–7, Jan. 1984. [8] D. F. Morrison, Multivariate Statistical Methods. New York: McGrawHill, 1990, pp. 313–317. [9] S. Krupenin, “Physical mechanisms limiting the manufacturing yield of millimeter-wave power InP HEMTs,” B.S. thesis, Mass. Inst. Technol., Cambridge, 1998. [10] M. H. Somerville and J. A. del Alamo, “A model for tunneling-limited breakdown in high-power HEMTs,” in IEDM Tech. Dig., 1996, pp. 35–38.

KRUPENIN et al.: MANUFACTURING UNIFORMITY OF MILLIMETER-WAVE POWER InP HEMT’s

[11] H. Rohdin et al., “Semi-analytical analysis for optimization of 0.1- m InGaAs-channel MODFET’s with emphasis on on-state breakdown and reliability,” in Proc. Int. Conf. InP and Related Materials, 1997, pp. 357–360. [12] D. R. Greenberg and J. A. del Alamo, “Velocity saturation in the extrinsic device: A fundamental limit in HFETs,” IEEE Trans. Electron Devices, vol. 41, pp. 1334–1339, Aug. 1994. [13] J. Elliott et al., “A flexible 3-inch fabrication line for InP-based HEMT and HBT MMIC production,” in Proc. Int. Conf. InP and Related Materials, 1997, pp. 501–504.

S. Krupenin received the B.S. degree in physics from the Massachusetts Institute of Technology (MIT), Cambridge, in 1998, and the dual M.S. degrees in electrical engineering and engineering management, both from Stanford University, Stanford, CA, in 2000. He plans to pursue doctoral research in RF CMOS design at Stanford. He has been an RF Engineer in the Wireless Broadband Networks Division, Lucent Technologies.

Roxann R. Blanchard (M’99) received the B. S. degree in electrical engineering from the University of Vermont, Burlington, in 1989, and the M.S. and Ph.D. degrees in electrical engineering from the Massachusetts Institute of Technology (MIT), Cambridge, in 1994 and 1999, respectively. Her Ph.D. work included the study and fabrication of InP-channel and InGaAs-channel InP HEMT’s. In addition, she examined the effects of hydrogen exposure on InGaAs/InAlAs HEMT’s and GaAs PHEMT’s. From 1989 to 1994, she worked at Raytheon Company, Sudbury, MA, developing radiation-hardened CMOS and Bi CMOS processes. While at MIT, she designed a complementary Si-biplar process, optimized for implementing an adiabatic logic technology, Recovered Energy Logic.

1565

M. H. Somerville, photograph and biography not available at the time of publication.

Jesus A. del Alamo (SM’92) received the degreee of Telecommunications Engineer from the Polytechnic University of Madrid, Spain, in 1980, and the M.S. and Ph.D. degrees in electrical engineering from Stanford University, Stanford, CA, in 1983 and 1985, respectively. He carried out his Ph.D. dissertation on minority carrier transport in heavily doped silicon. From 1977 to 1981, he was with the Institute of Solar Energy, Polytechnic University of Madrid, working on silicon solar cells. From 1985 to 1988, he was a Research Engineer with NTT LSI Laboratories, Atsugi, Japan, where he conducted research on III-V heterostructure field-effect transistors. Since 1988, he has been with the Department of Electrical Engineering and Computer Science, Massachusetts Institute of Technology (MIT), Cambridge, where he is currently Professor. His current research interests are in gigahertz power transistors: Si LDMOS on SOI, GaAs PHEMT’s and InP HEMT’s. Dr. del Alamo was an NSF Presidential Young Investigator from 1991 to 1996. In 1992, he was awarded the Baker Memorial Award for Excellence in Undergraduate Teaching at MIT. In 1993, he received the H. E. Edgerton Junior Faculty Achievement Award at MIT.

K. G. Duh, photograph and biography not available at the time of publication.

P. C. Chao (SM’91), photograph and biography not available at the time of publication.

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 8, AUGUST 2000

Physical Mechanisms Limiting the Manufacturing Uniformity of Millimeter-Wave Power InP HEMT’s S. Krupenin, Roxann R. Blanchard, Member, IEEE, M. H. Somerville, Jesus A. del Alamo, Senior Member, IEEE, K. G. Duh, and P. C. Chao, Senior Member, IEEE

Abstract—We have developed a methodology to diagnose the physical mechanisms limiting the manufacturing uniformity of millimeter-wave power InAlAs/InGaAs HEMT’s on InP. A statistical analysis was carried out on dc figures of merit obtained from a large number of actual devices on an experimental wafer. correlation studies and principal component analysis of the results indicated that variations in Si delta-doping concentration introduced during molecular-beam epitaxy accounted for more than half of the manufacturing variance. Variations in the gate-source distance that is determined by the electron-beam alignment in the gate formation process were found to be the second leading source of manufacturing variance. The statistical methodology used in this work is suitable for continuous process yield diagnostics and improvement in a manufacturing environment.

I. INTRODUCTION

T

HE InP high electron mobility transistor (HEMT) is the leading contender for high-power high-efficiency millimeter-wave power amplifiers [1], [2]. As the InP HEMT technology matures, manufacturing issues come to the foreground. To date there has been little work on understanding the key factors affecting the manufacturing uniformity of these devices. Such a study has been hampered by the considerable amount of work that it takes to measure millimeter-wave power figures of merit. Manufacturing uniformity control and improvement is critical because high cost represents a significant road block in the development of millimeter-wave systems. In this work we have carried out a statistical study of dc figures of merit of InP power HEMT’s that strongly impact the millimeter-wave performance of these devices. All of the selected figures of merit were measured in actual devices. A statistical analysis of the results using a principal components analysis (PCA) was carried out. This analysis was instrumental in revealing the two dominant physical sources of variability in these figures of merit. The methodology used in this work can be easily implemented in a manufacturing environment for continuous process diagnostics and improvement.

Manuscript received August 6, 1999; revised February 2, 2000. This work was supported by the MAFET program, through Sanders Lockheed Martin. The review of this paper was arranged by Editor A. S. Brown. S. Krupenin is with Stanford University, Stanford, CA 94305 USA. R. R. Blanchard is with Analog Devices Inc., Wilmington, MA 01887 USA. M. H. Somerville is with Vassar College, Poughkeepsie, NY 12604 USA. J. A. del Alamo is with the Massachusetts Institute of Technology, Cambridge, MA 02139 USA (e-mail: [email protected]). K. G. Duh and P. C. Chao are with Sanders Lockheed Martin, Nashua, NH 03061 USA. Publisher Item Identifier S 0018-9383(00)06032-9.

II. EXPERIMENTAL The devices studied in this work are 0.1 m gate length and 25 m gate width double-heterostructure InP power HEMT’s on one experimental 3-in wafer from Lockheed Martin Sanders [3], [4]. The heterostructure was grown by molecular-beam epitaxy (MBE) and includes two Si delta-doped layers above and below the channel. The devices feature an electron-beam written T-gate and a selectively recessed depleted cap. A total of 50 devices located on every other die of the wafer were studied. All figures of merit were measured with an identical probe configuration, allowing fast and completely automated measurements. We selected ten dc figures of merit that map to key millimeter-wave power figures of merit. They are listed in Table I. They include the threshold voltage, , the maximum transcon, the gate-source voltage at which ductance, occurs, , the maximum drain current, , the output conductance, , the off- and on-state breakdown and , and the source and voltages, and . The measurement conditions for drain resistances, these figures of merit are also summarized in Table I. Basically, and were obtained from the transfer characteristics. was obtained from two transfer char. and acteristics at two close values of were extracted using the drain-current injection technique [5]. was measured using the gate-current extraction techand were obtained using the end-resistance nique [6]. technique [7]. Of the 50 devices that were measured two were found to be anomalous and their corresponding data were discarded. Table I lists the mean and standard deviation of each figure of merit. The standard deviation as percentage of the mean is additionally given. Variations of the figures of merit never exceed 16% across the entire wafer. The correlation matrix of the measurements of the figures of merit is shown on Fig. 1. Each vignette lists the correlation coefficient between two figures of merit. A correlation coefficient close to one indicates a strong positive correlation between the two selected figures of merit; if close to 1, the correlation is strong but negative; if close to zero, the correlation is weak. Some of the correlation coefficients on Fig. 1 can be interpreted and exhibit a strong positive cordirectly. For example, relation coefficient of 0.68. This suggests a contact resistance or doping level control problem and excludes misalignment of the gate process from being a dominant source of variation in these figures of merit (it would result in a negative correlation coefficient). Spatial information is often useful in identifying sources of variability. Fig. 2 shows the spatial distribution across the wafer

0018–9383/00$10.00 © 2000 IEEE

KRUPENIN et al.: MANUFACTURING UNIFORMITY OF MILLIMETER-WAVE POWER InP HEMT’s

DEFINITIONS

Fig. 1.

AND THE

1561

TABLE I MEASURED VALUES OF THE DC FIGURES OF MERIT USED IN THIS WORK (L = 0:1 m, “STDV” REFERS TO THE STANDARD DEVIATION OF THE FIGURES OF MERIT

W = 25 m).

Correlations among dc figures of merit. The number in each vignette indicates the correlation coefficient.

of two figures of merit: and . While exhibits a circular symmetry, appears to show a linear gradient from left to right in the figure. This suggests that there are at least two different and independent mechanisms at play that result in variations in the figures of merit. From examination of the data in Figs. 1 and 2 alone, it is not possible to uncover the physical sources of variability. In order

to further our insight into the physics underlying variations in the figures of merit we have performed PCA of the data. III. PRINCIPAL COMPONENT ANALYSIS PCA is a statistical technique that performs a coordinate transformation from the original space of electrical measure-

1562

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 8, AUGUST 2000

Fig. 2. Spatial distribution on the wafer of BV and g . The fact that these two distributions are very different suggests that there are at least two major mechanisms that result in manufacturing variations. Fig. 4. Contributions of each of the principal components to the variance of each dc figure of merit. The signs indicate whether a component has a positive or negative correlation with a given figure of merit (see text).

Fig. 3. Relative importance of the principal components in the manufacturing variance. P1 explains 51% of the variance of the manufacturing process.

ments to a new space of uncorrelated “principal components.” These principal components are ordered according to the total variance that they account for in the original data: first P1 is selected to account for the maximum possible variance in the data set, then the second component, P2, is selected to maximize the variance of the residual after P1 is removed, and so on. A comprehensive treatment of PCA can be found in [8]. More details about the use of PCA in our work can be found in [9]. In the first pass, all figures of merit were weighted equally. Emphasis on selected figures of merit can be made by introducing appropriate weights. The relative contribution of each principal component to the total variance of the data set is shown in Fig. 3. This figure shows that the most significant component, P1, accounts for 51% of the total variance of the process. Correct identification of this component followed by appropriate corrective action can significantly improve the manufacturing uniformity of this process. The second and the third components account for 21% and 13% of the total variance respectively. The rest of the components add up to a total of 15%. 80% confidence intervals for the contributions of each principal component can be found as in [8]. They are listed in brackets in Fig. 3. P1, for example, accounts with 80% confidence for 41% to 69% of the variance of the entire data set. The confidence intervals of components P5 through P10 overlap badly. This indicates that the experimental data is

insufficient for computing their values and identifying them. Identification and correction of the first three components, however, is sufficient for dramatic uniformity improvement. In order to carry out the identification of the leading principal components, their relative impact on each dc figure of merit should be examined. Fig. 4 shows a percentage of the variance of each figure of merit that is attributed to each principal component. For example, P1 accounts for nearly 80% of the variance of . In contrast, P1 accounts for less than 25% of the variance , while P2 accounts for nearly 70% of it. P3 is seen of to enter strongly in the variance of . The percentages shown in Fig. 4 are statistically significant for each of the three most important components. The standard deviations of the contributions of the first three principal components toward any figure of merit did not exceed 9% under the assumption of a multivariate normal distribution [8]. Hence Fig. 4 is a reliable vehicle for physical identification of the three leading principal components. Fig. 4 also indicates the sign of the correlation between the principal components and the figures of merit. PCA does not yield the absolute signs of the correlations, just the relative sign among all correlations of a given principal component. For exhas a contrary sign to ample, the correlation between P1 and . In Fig. 4, a choice of signs has the correlation of P1 and been made that makes physical sense and that aids the identification of the physical origin of the principal components. This is discussed in detail below. Spatial distributions of the principal components can also be constructed. They are exhibited on Fig. 5 for P1, P2 and P3. The circular symmetry of P1 and the linear gradient distributions of P2 and P3 offer further clues for their identification. This figure also shows how these three principal components are uncorrelated: their spatial distributions are very different. We now proceed to give a physical interpretation to P1, P2 and P3. The previous section suggests that these principal components are closely related to various steps of the manufacturing process. The identification is facilitated by Fig. 4, which indicates the nature of relationships between the principal components and the figures of merit.

KRUPENIN et al.: MANUFACTURING UNIFORMITY OF MILLIMETER-WAVE POWER InP HEMT’s

Fig. 5. Spatial distributions on the wafer of the first three principal components. Notice that the first component, P1, has a radial distribution, while P2 and P3 exhibit linear gradients along orthogonal directions.

A. Interpretation of P1 Fig. 4 shows that P1 has a strong positive correlation with and strong negative correlations with , the breakdown voltages, and the parasitic resistances. This behavior can only be explained by associating P1 with the sheet carrier concentration in the channel of the device, . Let us examine this hypothesis in detail. • P1 accounts for 78% of the variance in , and the correlaincreases the inversion charge tion is negative. Higher more negin the channel in equilibrium which makes ative. is large (77%) and positive. • The impact of P1 on in InP power This is consistent with the fact that [11]. HEMT’s is limited by • P1 has a relatively large impact on the variances of all three breakdown voltages, and the correlation between P1 and these quantities is negative. It is well known that all is increased these breakdown voltages decrease when [4], [10]. P1 accounts for a substantial fraction of the variance of and and exhibits a negative correlation. This is also consistent with P1 being related to in the channel since and is the access resistance from the a portion of edge of the ohmic contact to the edge of the gate. Additionally, this is a power device design with a surface depleted cap in which the access resistance is dominated by . • P1 has a small but positive correlation with the variance of . This is also consistent with the identification of P1 is the extrinsic transconductance as related to . increases through and it should increase slightly when on . the negative impact of The negative correlation between P1 and can be explained through the impact of on . As increases, shifts down and with it the whole vs. curve shifts to lower voltages, thus decreasing . and P1 stems from • The positive correlation between the fact that increases with the bias current at which it as discussed is measured which in turn increases with above. The preceeding discussion makes it quite convincing that P1 is directly associated with the sheet carrier concentration of change? There electrons in the channel, . But what makes

1563

are two possibilities for it, one is the InAlAs insulator thickness, the second one is the Si doping level in the delta-doped supply layers. The weak correlation between P1 and allows us to rule out the first option since a change in insulator thickness should strongly affect the transconductance of the device through the insulator capacitance. Hence, P1 represents the Si doping level in the supply layers. The Si dopants are introduced during the MBE growth of the structure in the form of two delta-doped layers above and below the channel. The sample is rotated during MBE growth in order to compensate for spatial nonuniformity of the Si flux emanating from the effusion cell. This compensation is not perfect and a variation of Si concentration with a circular symmetry results on the wafer. This is precisely what is observed for the spatial distribution of P1 over the wafer shown in Fig. 5. B. Interpretation of P2 P2 has a positive correlation with , but only a weak influ(Fig. 4). Its impact on is very large (63%), ence on but there is none on . There is also negligible influence of P2 on . This strongly suggests that P2 is related to the gatesource extrinsic region of the device. A likely explanation for the correlation of P2 with the figures of merit is the identifica. tion of P2 with the variations in the gate-source distance Let us examine this hypothesis in detail. , because does not • P2 has a negligible impact on depend on the position of the source contact relative to the gate. arises through • The negative correlation of P2 and , which is directly affected by . and • The negative correlations between P2, are related. The peak and subsequent drop in transconductance in the devices under test results from the blow up of source resistance at high current values due to velocity saturation [12]. A higher value of makes this condition occur at smaller values of current, and . thus leading to a smaller • As an extrinsic source related parameter, P2 should have no impact on and the breakdown voltages. makes sense • The positive correlation between P2 and is linearly proportional to . since is related to and that in turn is • In principle, since , one would expect a negative correlation affected by and P2: the higher , the smaller and between ought to be. This is not observed in our results. There and is no statistically significant correlation between P2. A possible explanation for this is that these are asymmetric devices with the gate placed closer to the source. Thus, the relative impact of misplacing the gate is significantly higher on the source side than on the drain side. Additionally, asymmetric gate placement makes the imthan , as observed in pact of variations higher in Fig. 4. This makes it harder to identify any other sources . of variance in Gate-source distance variations are determined by the reproducibility of the positioning of the electron beam process used to write the gate. P2 has a roughly linear distribution on the wafer

1564

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 8, AUGUST 2000

Fig. 6. Identity of the first two principal components in the structure of an InP power HEMT.

(Fig. 5). This is consistent with the identification of P2 as an electron-beam process related variable, since the electron beam draws the gate on the wafer scanning the die in a linear manner. Fig. 6 shows a schematic diagram of the device indicating the physical origin of P1 and P2. C. Interpretation of P3 , The results of Fig. 4 indicate that P3 affects only . This suggests a strong association of P3 with the exand trinsic drain portion of the device. Upon detailed examination of all correlations and their signs, no single structural parameter of the device could be found that is consistent with all results. The detailed origin of P3 remains unknown. IV. DISCUSSION Measurements on transmission line model (TLM) test structures were carried out in an effort to confirm the identity of P1. The saturation current that is obtained in a TLM structure when a relatively high voltage is applied is directly proportional to and the electron saturation velocity . Since is set by the nature of the material, it should not be affected by small manufacturing variations. Hence, the maximum current in a TLM constitutes a direct probe of the sheet carrier concentration in the channel of a HEMT with a depleted cap. The TLM’s used in this work were 100 m wide and 50 m long. The saturation current was measured at 10 V in every die in which transistor measurements had been performed. Fig. 7 , as a shows the obtained maximum current in each TLM, function of the value of P1 for every die. There is a very close correlation across the entire wafer in these two parameters: the correlation coefficient is 0.84. In consequence, this measurement constitutes an independent confirmation of the identification of P1 as the Si delta-doping concentration with a direct immade earlier. pact on the sheet carrier concentration Our findings are in substantial agreement with those of Elliott et al. [13] on TRW’s 3-in fabrication line for InP-based HEMT and HBT MMIC’s. These authors single out MBE growth as the most critical node in InP HEMT MMIC production. This is in agreement with the MBE origin of P1 in our work. Additionally, they identified gate formation as the second most critical node for HEMT’s. They found that gate length and gate-source spacing are critical parameters. While we have not been able to isolate the impact of the gate length variations, we relate P2 to

Fig. 7. Maximum current through a TLM test structure versus the P1 value for the HEMT device on the same die. The correlation coefficient is 0.84.

the distance between the gate and the source, in agreement with the findings in [13]. V. CONCLUSION In summary, we used PCA to identify the two most important sources of manufacturing variability in InP power HEMT’s: the concentration of Si dopants in the delta-doping layers of the device and the distance between the gate and the source. Jointly these two components account for 72% of manufacturing variations in this process. Our findings are in agreement with those reported by Elliott et al. [13] on TRW’s InP based MMIC fabrication line. Necessary statistical data were obtained from simple dc measurements on actual transistors—no specialized test structures were required. Our methodology can be easily implemented in a manufacturing environment for continuous process uniformity diagnostics and improvement. REFERENCES [1] P. M. Smith, “InP-HEMT’s for microwave and millimeter-wave applications,” in Int. Conf. InP and Related Materials, 1995, pp. 68–72. [2] J. A. del Alamo and M. H. Somerville, “Breakdown in millimeter-wave power InP HEMTs: A comparison with GaAs PHEMTs,” IEEE J. SolidState Circuits, vol. 34, pp. 1204–1211, Sept. 1999. [3] C. S. Putnam et al., “Temperature dependence of breakdown voltage in InAlAs/InGaAs HEMTs: Theory and experiments,” in Int. Conf. InP and Related Materials, 1997, pp. 197–200. [4] M. H. Somerville et al., “On-state breakdown in power HEMTs: Measurements and modeling,” in IEDM Tech. Dig., 1997, pp. 553–556. [5] S. R. Bahl and J. A. del Alamo, “A new drain-current injection technique for the measurement of breakdown voltage in FETs,” IEEE Trans. Electron Devices, vol. 40, pp. 1558–1560, Aug. 1993. [6] M. H. Somerville et al., “A new gate current extraction technique for measurement of on-state breakdown voltage in HEMTs,” IEEE Electron Device Lett., vol. 19, pp. 405–407, Nov. 1998. [7] K. Lee et al., “A new interpretation of “end” resistance measurements,” IEEE Electron Dev. Lett., vol. EDL-5, pp. 5–7, Jan. 1984. [8] D. F. Morrison, Multivariate Statistical Methods. New York: McGrawHill, 1990, pp. 313–317. [9] S. Krupenin, “Physical mechanisms limiting the manufacturing yield of millimeter-wave power InP HEMTs,” B.S. thesis, Mass. Inst. Technol., Cambridge, 1998. [10] M. H. Somerville and J. A. del Alamo, “A model for tunneling-limited breakdown in high-power HEMTs,” in IEDM Tech. Dig., 1996, pp. 35–38.

KRUPENIN et al.: MANUFACTURING UNIFORMITY OF MILLIMETER-WAVE POWER InP HEMT’s

[11] H. Rohdin et al., “Semi-analytical analysis for optimization of 0.1- m InGaAs-channel MODFET’s with emphasis on on-state breakdown and reliability,” in Proc. Int. Conf. InP and Related Materials, 1997, pp. 357–360. [12] D. R. Greenberg and J. A. del Alamo, “Velocity saturation in the extrinsic device: A fundamental limit in HFETs,” IEEE Trans. Electron Devices, vol. 41, pp. 1334–1339, Aug. 1994. [13] J. Elliott et al., “A flexible 3-inch fabrication line for InP-based HEMT and HBT MMIC production,” in Proc. Int. Conf. InP and Related Materials, 1997, pp. 501–504.

S. Krupenin received the B.S. degree in physics from the Massachusetts Institute of Technology (MIT), Cambridge, in 1998, and the dual M.S. degrees in electrical engineering and engineering management, both from Stanford University, Stanford, CA, in 2000. He plans to pursue doctoral research in RF CMOS design at Stanford. He has been an RF Engineer in the Wireless Broadband Networks Division, Lucent Technologies.

Roxann R. Blanchard (M’99) received the B. S. degree in electrical engineering from the University of Vermont, Burlington, in 1989, and the M.S. and Ph.D. degrees in electrical engineering from the Massachusetts Institute of Technology (MIT), Cambridge, in 1994 and 1999, respectively. Her Ph.D. work included the study and fabrication of InP-channel and InGaAs-channel InP HEMT’s. In addition, she examined the effects of hydrogen exposure on InGaAs/InAlAs HEMT’s and GaAs PHEMT’s. From 1989 to 1994, she worked at Raytheon Company, Sudbury, MA, developing radiation-hardened CMOS and Bi CMOS processes. While at MIT, she designed a complementary Si-biplar process, optimized for implementing an adiabatic logic technology, Recovered Energy Logic.

1565

M. H. Somerville, photograph and biography not available at the time of publication.

Jesus A. del Alamo (SM’92) received the degreee of Telecommunications Engineer from the Polytechnic University of Madrid, Spain, in 1980, and the M.S. and Ph.D. degrees in electrical engineering from Stanford University, Stanford, CA, in 1983 and 1985, respectively. He carried out his Ph.D. dissertation on minority carrier transport in heavily doped silicon. From 1977 to 1981, he was with the Institute of Solar Energy, Polytechnic University of Madrid, working on silicon solar cells. From 1985 to 1988, he was a Research Engineer with NTT LSI Laboratories, Atsugi, Japan, where he conducted research on III-V heterostructure field-effect transistors. Since 1988, he has been with the Department of Electrical Engineering and Computer Science, Massachusetts Institute of Technology (MIT), Cambridge, where he is currently Professor. His current research interests are in gigahertz power transistors: Si LDMOS on SOI, GaAs PHEMT’s and InP HEMT’s. Dr. del Alamo was an NSF Presidential Young Investigator from 1991 to 1996. In 1992, he was awarded the Baker Memorial Award for Excellence in Undergraduate Teaching at MIT. In 1993, he received the H. E. Edgerton Junior Faculty Achievement Award at MIT.

K. G. Duh, photograph and biography not available at the time of publication.

P. C. Chao (SM’91), photograph and biography not available at the time of publication.